Presentation on theme: "Presentation downloadable from www.tececo.com 1 Carbonating Mortars Abatement, Sequestration and Waste Utilization in the Built Environment Earthship Brighton."— Presentation transcript:
Presentation downloadable from 1 Carbonating Mortars Abatement, Sequestration and Waste Utilization in the Built Environment Earthship Brighton (UK) – The first building utilising TecEco eco-cement concretes and mortars In the first part of my talk I will discuss the requirements for carbonation in the context of mortars as this is poorly understood. I will then talk more generally about eco-cements in comparison to lime mortars John Harrison B.Sc. B.Ec. FCPA.
Presentation downloadable from 2 Introduction Carbonating mortars based on lime have traditionally held walling units together and are still the choice of many builders. The reintroduction of carbonating mortars represents and opportunity for abatement, waste utilisation and even net sequestration The requirements for proper carbonation when carbonating lime mortars or the new eco-cements magnesian cement mortars are used is poorly understood, especially in the English speaking world.
Presentation downloadable from 3 Introduction This presentation discusses the ramifications of physical factors such as aggregate size, grading and moisture and concludes that: –sands suitable for hydraulic cements are not suitable for carbonating cements and visa versa and –there are deficiencies in the current standards and codes of practice that do not recognize this. Eco-cements are then described
Presentation downloadable from 4 Carbonating Mortars Background Until the beginning of this century most buildings were constructed with lime and hydraulic lime mortars and many still stand as testament to their quality. –Examples include many Roman lime mortars such as in Hadrians wall built nearly 2000 years ago (122 AD) and the Tower of London built some 900 years ago. Portland cement until recently had taken over the mortar market in English speaking countries, whereas in many other parts of the world such as Slovenia where PC mortars are banned, lime mortars never went out of use.
Presentation downloadable from 5 Current Trends The focus is on ease of use by bricklayers rather than end result –For example in the most used 1:1:6 or 1:2:9 (pc, lime, aggregate) type mixes, the aggregates used are generally much too fine and well graded for the lime to serve as much other than a plasticiser. Little advantage is taken of pozzolanic wastes except in Europe, Asia and the USA. There is currently a trend back to the use of lime for mortars mainly for the plasticity introduced to mixes. With the advent of carbon taxes there could be a rush back to carbonating mortars driven by the taxes avoided or extra credits available
Presentation downloadable from 6 The Historic Record The historic record is confusing and a thorough analysis is overdue –based on fundamentals –that is not clouded by inappropriate standards. Although good mortars from the past have lasted through the ages there have also been many failures as well. Most old carbonating lime mortars are a mix of lime putty, lime sand, and grit. –Generally a greater proportion of lime was used for sandstone or sedimentary rocks and a harder mortar used for granite or impervious rocks. The biggest problem in trying to discern best practice from the past is that historic mortar formulations are many and varied although underlying many of them there exists some common lessons for the present that are in agreement with good science.
Presentation downloadable from 7 Roman Mortars The Romans had two distinct types of mortar* –One was made with simple lime and river sand, mixed at a ratio of three parts sand to one part lime. This was definitely a carbonating type –The other type used pozzolan instead of river sand and was mixed at a ratio of two parts pozzolan to one part lime This was probably at least partially hydraulic depending on the porosity *Benjamin Herring, editor in chief of constructor magazine
Presentation downloadable from 8 Roman Specifications The oldest record: Book II, chapter IV of the Ten Books of Architecture by Vitruvius Pollio. –According to Vitruvius the best (sand) will be found to be that which crackles when rubbed in the hand, while that which has much dirt in it will not be sharp enough. Again: throw some sand upon a white garment and then shake it out; if the garment is not soiled and no dirt adheres to it, the sand is suitable Vitruvious was talking about gritty sand with no fines. The 16th century architect Andrea Palladio is renowned for "The Four Books of Architecture –translated into English in the early 18th century –used as a principal reference for building for almost two centuries (Palladio, Isaac Ware translation, 1738). –In the first book Palladio says, "the best river sand is that which is found in rapid streams, and under water-falls, because it is most purged". In other words, it is coarse. Compare this with most sand for use in mortar today. The conclusion from history is that a coarse gritty sand that is not graded for minimum paste is required.
Presentation downloadable from 9 Advantages of Carbonating Mortars Modern Portland cement mortars and even some fully hydraulic lime mortars –Set too hard and do not self-heal. –Tend to crack with any movement and let water in. Once the water is in they are so tight they do not let it out again as they cannot breathe leading to further problems. Carbonating mortars: –Are more plasticity –Are much more forgiving. As all buildings move, especially those built pre 1900, many of which had less solid foundations, this property alone is reason enough to use them. A carbonating component is required for crystalline bridging of cracks that develop through movement. Global warming is a major issue and the huge potential in the built environment for sequestering carbon cannot be ignored. There is an urgent need to reconsider the merits of properly carbonating mortars in the context of global warming.
Presentation downloadable from 10 Advantages of Carbonating Cements for Mortars Sustainability with less net emissions The accommodation of minor and thermal movement without damage. The avoidance of expansion joints. Improved insulation and avoidance of cold bridging. Reduced risk of condensation. Low risk of salt staining. Alterations can be effected easily and masonry revised. Lower pH Masonry life is increased. Masonry can more easily be cleaned and reused. More resistant to freeze thaw and sulphate. Reduced calcium aluminate content & reactions with sulphate in stone. Lower alkalinity and reactions with stone, particularly sandstone Better bond to acidic or more neutral rocks like sandstone. Buildings which themselves breathe are healthier to live in.
Presentation downloadable from 11 Alledged Disadvantages of Carbonating Mortars and Cements Lea (The Chemistry of Cement and Concrete) Mortar taken from buildings many hundreds of years old, if uninjured, is found to consist mainly of calcium hydroxide, only the external portion has been converted to carbonate. –Note however that the lack of carbonation of some old mortars can be explained as a function of low porosity due to poor aggregate selection rather than due to an innate inability of lime to carbonate. Lime type carbonating mortars are considered by many as too weak for copings, chimneys and other exposed work. –As minerals such as nesquehonite found in eco- cement mortars are micro structurally stronger this problem is overcome by substitution with magnesia as in eco-cements.
Presentation downloadable from 12 Alledged Disadvantages of Carbonating Mortars and Cements Currently there is also a danger regarding use in frost prone months. –This is however not the fault of the binder so much as because the fine sands used not only dont let air in for carbonation – they dont let moisture out. Lime mortars are subject to attack by acid rain. –True. Fortunately however eco-cement mortars appear to be much more acid resistant. The thermodynamics and kinetics is complex however the evidence is that no potholing or caving is ever found in magnesium carbonate country. Chlorides and sulphates attack lime and Portland cement mortars –True. Fortunately chlorides and sulphates are rendered chemically inactive and cementitiously useful by the magnesia in eco-cement type formulations. As these salts are common in some rocks and bricks and certainly in city environments, particularly near the sea or where salt is used on roads, eco-cements should be considered for this reason alone.
Presentation downloadable from 13 Eco-Cements Get over Many of the Disadvantages The new magnesian eco-cements developed by TecEco –set by absorbing carbon dioxide in porous substrates such as mortars and concrete blocks –are easier to use –do not appear to suffer the segregation problem of mixed lime PC mortars –potentially develop greater strengths including bond strength to bricks because of the unique microstructure attributable to the highly acicular nature of the hydrated magnesium carbonates formed. –develop higher early tensile strengths –are more acid resistant –retain the benefits of self healing attributed to lime mortars. –are more acid resistant –Are very plastic –Are more efficient as more binder is produced for a given weight of eco-cement. –And carbonate absorbing CO 2
Presentation downloadable from 14 Carbonating Cements and Sequestration Cementitious materials that go the full thermodynamic cycle gaining strength by carbonation offer tremendous potential because the CO 2 chemically released during manufacture can be recaptured resulting in significant overall sequestration. –To put the tonnages involved into context, in 2004, by calculation from clay brick and concrete block production, Australians used about 300,000 tonnes of Portland cement to make mortars. Roughly only 25% of this cement carbonates so 225,000 tonnes of CO 2 are released assuming emissions are taken to be roughly one tonne of CO 2 per tonne of cement. If lime or high magnesian eco-cements were used in Australia for mortars the reduction in CO 2 emissions would be a significant 225,000 tonnes. Australia is only about 1.4% of the economic world so globally the figure is significant.
Presentation downloadable from 15 Other Sustainable Benefits of Carbonating Cements The bulk density is lower than Portland cement enabling fuel savings during distribution. Buildings constructed with all but the strongest lime and eco-cements can also easily be altered and recovered masonry reused or in the case of eco-cement blocks, recycled. –In contrast bricks held together with Portland cement mortars usually cannot easily be recycled as the mortar is too strong. The production of bricks and masonry units is an energy intensive process and the savings involved as a result of more efficient recycling would be considerable.
Presentation downloadable from 16 Preparing for Sequestration There will potentially be a rush towards carbonating cements as carbon credits became available for proven sequestration The cement industry needs to prepare itself for such a commercial opportunity. –Learn to understand the differing requirements of carbonating cements of varying degrees of hydraulicity and carbonation potential. –Develop performance standards that recognise these differing requirements.
Presentation downloadable from 17 Performance Based Standards are Needed Lime mortar standards were developed at the time that Portland cement was being introduced as a key material in mortars. –As a consequence most of the curing conditions were established on the basis of the hydration requirements of Portland cement (minimum paste for cover) rather than the requirements of carbonation. It should be obvious that lime mortars cannot perform as well under these conditions. For example: –Mechanical testing at 28 days. Lime and eco-cement mortars take longer. Lime mortars require carbon dioxide for the carbonation reaction. –Although the presence of moisture will facilitate the carbonation reaction of the lime and crystallization of the resulting calcite crystals, too much moisture, as under the BS conditions, will slow down the reaction. –This can be explained by considering that all the exposed surfaces of the lime mortar are covered with a layer of liquid water and that the CO 2 has to diffuse through it before it can reach the lime surface.
Presentation downloadable from 18 Carbonation Requires the Right Sands & Aggregates The major problem with nearly all mortars today is that the same sands tend to be used for all of them regardless of the incongruous requirements for proper compaction or carbonation. Carbon dioxide is pervasive in the atmosphere at about 380 ppm (2005) and rising. –For carbonation to occur in either lime, blended lime PC or eco-cement mortars the mortar must be able to breathe. By breathing vapors must be able to pass into the mortar through it and out of it. –Carbonation reactions however generally occur in the aqueous phase much more quickly than in the gas phase and thus water vapor is also necessarily present. For porosity, a lack of fine fractions is required in the aggregates used and this is unfortunately poorly understood except by some in the restoration industry. In contrast, for Portland cement mortars to gain strength the main requirement is for a low water binder ratio. –For this relatively fine sands that are rounded and compact well are required that minimise the amount of cement required for full cover.
Presentation downloadable from 19 The Right Sands & Aggregates (2) The right sands should be clean and well graded, ranging lacking in fines and be gritty in texture. –Generally specify washed sharp sand with 3-4 mm grit (where the joints allow) and a low proportion of fines is suitable The coarsest grains should however be no more than 1/3 the depth of the mortar between bricks for easy laying. Beware of artificially crushed stone dusts (especially limestone). –Some say these cause shrinkage problems, are weak and have poor adhesion. Although logical as a ramification of the chemistry the requirements of sand aggregate seems to be poorly understood except by a few within the restoration fraternity
Presentation downloadable from 20 Particles Size Specification in Standards Jordan, J.W. The Conservation and Strengthening of Masonry Structures. in Proceedings of the 7th Australasian Masonry Conference Newcastle, New South Wales, Australia: University of Newcastle, Australia. Sand grading for permeable mortar compared to BS 1200 and AS recommendations (Note that a mortar for successful carbonation barely falls within the ranges specified by the standards. A more suitable mortar would most likely fall without.)
Presentation downloadable from 21 Improving The Status Quo One has to consider why in the face of science and the historic record the standards allow the use of such inappropriate aggregates for carbonation and apply such unfair advantages in tests to hydraulic cements. Perhaps the answer lies in a misguided belief that –the only binder is Portland cements and that the only sand sold should minimise paste required and optimise hydraulic setting. It is time cement companies dropped the philosophy of if its grey its great and all we make goes out the gate. –A small number are now making lime as well as Portland cement –A small number are now involved in geopolymers – The only enduring business is the business of change. The cement industry are in the mineral composite business and diversification could actually be more profitable, particularly if there were opportunities for carbon credits through sequestration in the built environment. –Adopting new technologies will result in new products and may mean new resources are defined many of which are wastes. New products create new market space. Pilzer, P.Z., Unlimited Wealth - The Theory and Practice of Economic Alchemy. 1 ed. 1990: Crown Publishers
Presentation downloadable from 22 Eco-Cements and the Sustainability Challenge There are new demands for sustainability being placed upon the industry. With the advent of Kyoto as a treaty there could even be money to be made from carbon credits if mortars containing lime or magnesia (as in eco-cements) were allowed to carbonate properly. The new eco-cements from TecEco are exciting as they are potentially better products that are far more sustainable. –They contain relatively high proportions of MgO that will first hydrate and then carbonate. –The production of magnesia can be achieved using an efficient low temperature process that can use waste heat or free solar energy. The capture of CO2 during this process would result in sequestration on a massive scale. The magnesia used is relatively fine and like lime, markedly improves rheology. Eco-cement mortars work well with some clays –Actually exhibiting more strength in their presence and this could be an advantage in terms of being able to utilise sands without the cost of washing and disposal problems associated with the clay fines fraction. –For mortar manufacture using wastes such as quarry fines this is an advantge. A case study on mud bricks using a high clay soil is on the TecEco web site.
Presentation downloadable from 23 Eco-Cements Eco-cements are similar but potentially superior to lime mortars because: –The calcination phase of the magnesium thermodynamic cycle takes place at a much lower temperature and is therefore more efficient. –Magnesium minerals are generally more fibrous and acicular than calcium minerals and hence add microstructural strength. Water forms part of the binder minerals that forming making the cement component go further. In terms of binder produced for starting material in cement, eco- cements are much more efficient. Magnesium hydroxide in particular and to some extent the carbonates are less reactive and mobile and thus much more durable.
Presentation downloadable from 24 Eco-Cements and the Sustainability Challenge Because Mg++ is a small and highly charged ion it tends to cause polar water molecules to orientate in layers around it introducing a shear thinning property improving for example anti sag properties in mortars as would methyl cellulose. Nesquehonite is the main observable carbonate and forms star like acicular growths which adds to microstructural strength. Fibrous carbonate growth may also improve bonding with brick, tiles and various walling substrates. Significant quantities of binder are produced. –The larger proportion of magnesium carbonates formed is CO 2 and water. In terms of binder produced for starting material in cement, eco- cements are nearly six times more efficient.
Presentation downloadable from 25 Eco-Cement Strength Development Eco-cements gain early strength from the hydration of PC. Later strength comes from the carbonation of brucite forming an amorphous phase, lansfordite and nesquehonite. Strength gain in eco-cements is mainly microstructural because of –More ideal particle packing (Brucite particles at 4-5 micron are under half the size of cement grains.) –The natural fibrous and acicular shape of magnesium carbonate minerals which tend to lock together. More binder is formed than with calcium –Total volumetric expansion from magnesium oxide to lansfordite is for example volume 811%. Mg(OH) 2 + CO 2 MgCO 3.5H 2 O From air and water
Presentation downloadable from 26 Eco-Cement Mortar Strength Gain Curve Eco-cement bricks, blocks, pavers and mortars etc. take a while to come to the same or greater strength than OPC formulations but are stronger than lime based formulations.
Presentation downloadable from 27 Chemistry of Eco-Cements There are a number of carbonates of magnesium. The main ones appear to be an amorphous phase, lansfordite and nesquehonite. The carbonation of magnesium hydroxide does not proceed as readily as that of calcium hydroxide. – G o r Brucite to nesquehonite = kJ.mol-1 –Compare to G o r Portlandite to calcite = kJ.mol-1 The dehydration of nesquehonite to form magnesite is not favoured by simple thermodynamics but may occur in the long term under the right conditions. G o r nesquehonite to magnesite = 8.56 kJ.mol-1 –But kinetically driven by desiccation during drying. Reactive magnesia can carbonate in dry conditions – so keep bags sealed! For a full discussion of the thermodynamics see our technical documents. TecEco technical documents on the web cover the important aspects of carbonation.
Presentation downloadable from 28 Eco-Cement Reactions
Presentation downloadable from 29 Eco-Cement Micro-Structural Strength
Presentation downloadable from 30 Proof of Carbonation - Minerals Present After 18 Months XRD showing carbonates and other minerals before removal of carbonates with HCl in a simple Mix (70 Kg PC, 70 Kg MgO, colouring oxide.5Kg, sand unwashed 1105 Kg)
Presentation downloadable from 31 Proof of Carbonation - Minerals Present After 18 Months and Acid Leaching XRD Showing minerals remaining after their removal with HCl in a simple mix (70 Kg PC, 70 Kg MgO, colouring oxide.5Kg, sand unwashed 1105 Kg)
Presentation downloadable from 32 Eco-Cement Biomimicry During earth's geological history large tonnages of carbon were put away as limestone and other carbonates and as coal and petroleum by the activity of plants and animals. Sequestering carbon in magnesium binders and aggregates in the built environment mimics nature in that carbon is used in the homes or skeletal structures of most plants and animals. We all use carbon and wastes to make our homes! Biomimicry In eco-cement blocks and mortars the binder is carbonate and the aggregates are preferably wastes
Presentation downloadable from 33 CO 2 Abatement in Eco-Cements Eco-cements in porous products absorb carbon dioxide from the atmosphere. Brucite carbonates forming lansfordite, nesquehonite and an amorphous phase, completing the thermodynamic cycle. No Capture 11.25% mass% reactive magnesia, 3.75 mass% Portland cement, 85 mass% aggregate. Emissions.37 tonnes to the tonne. After carbonation. approximately.241 tonne to the tonne. Portland Cements 15 mass% Portland cement, 85 mass% aggregate Emissions.32 tonnes to the tonne. After carbonation. Approximately.299 tonne to the tonne..299 >.241 >.140 >.113 Bricks, blocks, pavers, mortars and pavement made using eco-cement, fly and bottom ash (with capture of CO 2 during manufacture of reactive magnesia) have 2.65 times less emissions than if they were made with Portland cement. Capture CO % mass% reactive magnesia, 3.75 mass% Portland cement, 85 mass% aggregate. Emissions.25 tonnes to the tonne. After carbonation. approximately.140 tonne to the tonne. Capture CO 2. Fly and Bottom Ash 11.25% mass% reactive magnesia, 3.75 mass% Portland cement, 85 mass% aggregate. Emissions.126 tonnes to the tonne. After carbonation. Approximately.113 tonne to the tonne. For 85 wt% Aggregates 15 wt% Cement Greater Sustainability
Presentation downloadable from 34 TecEco Technology in Practice - Whittlesea, Vic. Australia First Eco-cement mud bricks and mortars in Australia –Tested up twice as strong as the PC controls –Mud brick addition rate 2.5% –Addition rate for mortars 1:8 not 1:3 because of molar ratio volume increase with MgO compared to lime.
Presentation downloadable from 35 Earthship Brighton – First Building to Use Eco-Cements Throughout Conclusion As materials scientists we must do all we can to change the technology paradigms so that carbon and wastes become resources. TecEco are mimicking nature where the principle building materials for trees, animals and fish has been for millennia carbon Aubrey John Weston Harrison B.Sc. B.Ec. FCPA.